#------------------------------------------------------------------------------
#$Date: 2019-11-22 22:28:34 +0200 (Fri, 22 Nov 2019) $
#$Revision: 231431 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/32/4003210.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003210
loop_
_publ_author_name
'Boal, Ben W.'
'Schmidt, Joel E.'
'Deimund, Mark A.'
'Deem, Michael W.'
'Henling, Lawrence M.'
'Brand, Stephen K.'
'Zones, Stacey I.'
'Davis, Mark E.'
_publ_section_title
;
 Facile Synthesis and Catalysis of Pure-Silica and Heteroatom LTA
;
_journal_issue                   22
_journal_name_full               'Chemistry of Materials'
_journal_page_first              7774
_journal_paper_doi               10.1021/acs.chemmater.5b03579
_journal_volume                  27
_journal_year                    2015
_chemical_formula_moiety         '0.08(O24 Si12)'
_chemical_formula_sum            'O2 Si'
_chemical_formula_weight         60.09
_space_group_crystal_system      cubic
_space_group_IT_number           221
_space_group_name_Hall           '-P 4 2 3'
_space_group_name_H-M_alt        'P m -3 m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2015-07-18
_audit_creation_method
;
Olex2 1.2
(compiled 2015.01.26 svn.r3150 for OlexSys, GUI svn.r4998),
 SHELXL-2014,
 and manual edit
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            24
_cell_length_a                   11.857(4)
_cell_length_b                   11.857(4)
_cell_length_c                   11.857(4)
_cell_measurement_reflns_used    9976
_cell_measurement_temperature    100
_cell_measurement_theta_max      57.17
_cell_measurement_theta_min      2.43
_cell_volume                     1667.0(10)
_computing_cell_refinement       'SAINT V8.34A (Bruker-AXS, 2007)'
_computing_data_collection       'APEX2 2014.11-0 (Bruker-AXS, 2007)'
_computing_data_reduction        'SAINT V8.34A (Bruker-AXS, 2007)'
_computing_molecular_graphics    'DIAMOND 3 (Crystal Impact, 1999)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_computing_structure_solution    'XT-2014/4 (Sheldrick, 2012)'
_diffrn_ambient_temperature      100
_diffrn_detector                 'CMOS Area Detector'
_diffrn_detector_area_resol_mean 10.24
_diffrn_detector_type            'Bruker PHOTON 100 CMOS'
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.978
_diffrn_measurement_device       'κ-geometry diffractometer'
_diffrn_measurement_device_type  'Bruker D8 VENTURE Kappa Duo PHOTON 100 CMOS'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  'multilayer mirrors'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0861
_diffrn_reflns_av_unetI/netI     0.0439
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.978
_diffrn_reflns_limit_h_max       27
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       23
_diffrn_reflns_limit_l_min       -27
_diffrn_reflns_number            48084
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.978
_diffrn_reflns_theta_full        25.000
_diffrn_reflns_theta_max         60.181
_diffrn_reflns_theta_min         2.429
_diffrn_source                   'I\mS HB micro-focus sealed tube'
_diffrn_source_current           1
_diffrn_source_power             0.05
_diffrn_source_type              'Incoatech I\mS HB'
_diffrn_source_voltage           50
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.540
_exptl_absorpt_correction_T_max  1.0000
_exptl_absorpt_correction_T_min  0.8962
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS-2014/5 (Sheldrick, 2014)'
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    1.437
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cube
_exptl_crystal_F_000             720
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.10
_refine_diff_density_max         1.530
_refine_diff_density_min         -0.750
_refine_diff_density_rms         0.117
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.152
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     21
_refine_ls_number_reflns         2479
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.152
_refine_ls_R_factor_all          0.0850
_refine_ls_R_factor_gt           0.0449
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0368P)²+0.2991P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0833
_refine_ls_wR_factor_ref         0.0933
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1731
_reflns_number_total             2479
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            cm5b03579_si_004.cif
_cod_data_source_block           p15229
_cod_original_cell_volume        1667.0(17)
_cod_database_code               4003210
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_max   0.948
_shelx_estimated_absorpt_t_min   0.948
_exptl_absorpt_special_details
;
SADABS-2014/5 (Bruker,2014/5) was used for absorption correction.
wR2(int) was 0.0668 before and 0.0588 after correction.
The Ratio of minimum to maximum transmission is 0.8962.
The λ/2 correction factor is 0.00150.
;
_olex2_refinement_description
;
;
_shelx_shelxl_version_number     2014/7
_olex2_submission_special_instructions 'No special instructions were received'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z'
'-x, y, -z'
'x, -y, -z'
'z, x, y'
'z, -x, -y'
'-z, -x, y'
'-z, x, -y'
'y, z, x'
'-y, z, -x'
'y, -z, -x'
'-y, -z, x'
'y, x, -z'
'-y, -x, -z'
'y, -x, z'
'-y, x, z'
'x, z, -y'
'-x, z, y'
'-x, -z, -y'
'x, -z, y'
'z, y, -x'
'z, -y, x'
'-z, y, x'
'-z, -y, -x'
'-x, -y, -z'
'x, y, -z'
'x, -y, z'
'-x, y, z'
'-z, -x, -y'
'-z, x, y'
'z, x, -y'
'z, -x, y'
'-y, -z, -x'
'y, -z, x'
'-y, z, x'
'y, z, -x'
'-y, -x, z'
'y, x, z'
'-y, x, -z'
'y, -x, -z'
'-x, -z, y'
'x, -z, -y'
'x, z, y'
'-x, z, -y'
'-z, -y, x'
'-z, y, -x'
'z, -y, -x'
'z, y, x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
Si1 Si 0.5000 0.86918(2) 0.31655(2) 0.00378(4) Uani 1 2 d S T P
O1 O 0.5000 0.79613(4) 0.20387(4) 0.00676(10) Uani 1 4 d S T P
O2 O 0.61064(4) 0.84036(6) 0.38936(4) 0.01360(11) Uani 1 2 d S T P
O3 O 0.5000 1.0000 0.28299(7) 0.01389(15) Uani 1 4 d S T P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
0.00 0.00 -1.00 0.0270
0.00 0.00 1.00 0.0490
0.00 1.00 0.00 0.0260
0.00 -1.00 0.00 0.0490
1.00 0.00 0.00 0.0490
-1.00 0.00 0.00 0.0330
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Si1 O2 109.57(3) . .
O1 Si1 O2 109.57(3) . 28_655
O1 Si1 O3 108.57(4) . .
O2 Si1 O2 109.43(5) 28_655 .
O3 Si1 O2 109.84(3) . 28_655
O3 Si1 O2 109.84(3) . .
Si1 O1 Si1 155.91(5) . 42_566
Si1 O2 Si1 146.27(4) 46_656 .
Si1 O3 Si1 151.22(6) . 2_675
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Si1 O1 1.5922(6) .
Si1 O2 1.6072(6) 28_655
Si1 O2 1.6072(6) .
Si1 O3 1.6014(6) .
O1 Si1 1.5922(6) 42_566
O2 Si1 1.6072(6) 46_656
O3 Si1 1.6014(6) 2_675
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O1 Si1 O2 Si1 176.06(8) . 46_656
O1 Si1 O3 Si1 180.000(0) . 2_675
O2 Si1 O1 Si1 60.03(3) . 42_566
O2 Si1 O1 Si1 -60.04(3) 28_655 42_566
O2 Si1 O2 Si1 -63.78(11) 28_655 46_656
O2 Si1 O3 Si1 60.20(3) 28_655 2_675
O2 Si1 O3 Si1 -60.20(3) . 2_675
O3 Si1 O1 Si1 180.000(0) . 42_566
O3 Si1 O2 Si1 56.88(10) . 46_656
